#------------------------------------------------------------------------------
#$Date: 2020-01-28 01:19:45 +0200 (Tue, 28 Jan 2020) $
#$Revision: 247263 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/00/34/4003469.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4003469
loop_
_publ_author_name
'Solokha, Pavlo'
'Eremin, Roman A.'
'Leisegang, Tilmann'
'Proserpio, Davide M.'
'Akhmetshina, Tatiana'
'Gurskaya, Albina'
'Saccone, Adriana'
'De Negri, Serena'
_publ_section_title
;
 New Quasicrystal Approximant in the Sc--Pd System: From Topological Data
 Mining to the Bench
;
_journal_name_full               'Chemistry of Materials'
_journal_paper_doi               10.1021/acs.chemmater.9b03767
_journal_year                    2020
_chemical_formula_moiety         'Pd14.52 Sc36.98, 1(Pd), 18(Sc)'
_chemical_formula_sum            'Pd15.52 Sc54.98'
_chemical_formula_weight         4122.81
_space_group_crystal_system      orthorhombic
_space_group_IT_number           71
_space_group_name_Hall           '-I 2 2'
_space_group_name_H-M_alt        'I m m m'
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   14.2722(7)
_cell_length_b                   14.3714(7)
_cell_length_c                   14.7878(7)
_cell_measurement_reflns_used    2550
_cell_measurement_temperature    295(2)
_cell_measurement_theta_max      31.795
_cell_measurement_theta_min      1.976
_cell_volume                     3033.1(3)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      295(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.975
_diffrn_measurement_device_type  'Bruker APEXII'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0320
_diffrn_reflns_av_unetI/netI     0.0155
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.975
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            36639
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.975
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         31.795
_diffrn_reflns_theta_min         1.976
_exptl_absorpt_coefficient_mu    10.073
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Bruker SADABS'
_exptl_crystal_colour            'metallic luster'
_exptl_crystal_density_diffrn    4.504
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'irregularly shaped'
_exptl_crystal_F_000             3732
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.04
_exptl_transmission_factor_max   0.7463
_exptl_transmission_factor_min   0.6107
_refine_diff_density_max         1.578
_refine_diff_density_min         -2.005
_refine_diff_density_rms         0.229
_refine_ls_goodness_of_fit_ref   1.093
_refine_ls_matrix_type           full
_refine_ls_number_parameters     126
_refine_ls_number_reflns         2796
_refine_ls_number_restraints     25
_refine_ls_restrained_S_all      1.088
_refine_ls_R_factor_all          0.0280
_refine_ls_R_factor_gt           0.0245
_refine_ls_shift/su_max          0.024
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0273P)²+22.1197P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0577
_refine_ls_wR_factor_ref         0.0591
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2550
_reflns_number_total             2796
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            cm9b03767_si_005.cif
_cod_data_source_block           shelx_CSD-1874073
_cod_database_code               4003469
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Pd1 Pd 0.0000 0.0000 0.0000 0.00910(11) Uani 1 8 d S T P A .
Pd2 Pd 0.33560(2) 0.20626(2) 0.0000 0.01180(7) Uani 1 2 d S T P A .
Pd3 Pd 0.0000 0.33423(2) 0.21002(2) 0.01276(7) Uani 1 2 d S T P A .
Pd4 Pd 0.20347(2) 0.0000 0.33362(2) 0.01314(7) Uani 1 2 d S T P A .
Pd5 Pd 0.5000 0.0000 0.16129(3) 0.01615(10) Uani 1 4 d S T P A .
Sc1 Sc 0.17841(5) 0.10944(5) 0.0000 0.00920(13) Uani 1 2 d S T P A .
Sc2 Sc 0.0000 0.0000 0.35361(7) 0.00943(18) Uani 1 4 d S T P A .
Sc3 Sc 0.38016(7) 0.0000 0.0000 0.00947(18) Uani 1 4 d S T P A .
Sc4 Sc 0.0000 0.18171(5) 0.10583(5) 0.00906(13) Uani 1 2 d S T P A .
Sc5 Sc 0.11011(5) 0.0000 0.16815(5) 0.00910(13) Uani 1 2 d S T P A .
Sc6 Sc 0.11696(4) 0.17771(4) 0.28718(3) 0.01000(10) Uani 1 1 d . . . . .
Sc7 Sc 0.0000 0.32341(6) 0.39631(5) 0.01251(14) Uani 1 2 d S T P A .
Sc8 Sc 0.0000 0.37974(8) 0.0000 0.01084(19) Uani 1 4 d S T P A .
Sc9A Sc 0.3878(12) 0.3792(11) 0.0000 0.012(4) Uani 0.44(3) 2 d S TU P A 1
Sc9B Sc 0.367(2) 0.3938(17) 0.0000 0.013(3) Uani 0.27(3) 2 d S TU P A 2
Sc9C Sc 0.4093(17) 0.370(2) 0.0000 0.010(2) Uani 0.29(3) 2 d S TU P A 3
Sc10 Sc 0.18707(4) 0.30113(4) 0.11127(4) 0.01071(10) Uani 1 1 d . . . . .
Sc11 Sc 0.30196(4) 0.11509(4) 0.17770(4) 0.01030(10) Uani 1 1 d . . . . .
Sc12 Sc 0.39766(6) 0.0000 0.32996(6) 0.01676(16) Uani 1 2 d S T P A .
Sc13 Sc 0.1857(11) 0.5000 0.0000 0.0163(16) Uani 0.49(4) 4 d S TU . A .
Pd23 Pd 0.2251(11) 0.5000 0.0000 0.0245(17) Uani 0.258(15) 4 d S TU . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Sc Sc 0.2519 0.3716 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pd Pd -0.9988 1.0072 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Sc5 Pd1 Sc5 64.59(3) 9 10
Sc5 Pd1 Sc5 115.41(3) 9 2
Sc5 Pd1 Sc5 180.00(3) 10 2
Sc5 Pd1 Sc5 180.0 9 .
Sc5 Pd1 Sc5 115.41(3) 10 .
Sc5 Pd1 Sc5 64.59(3) 2 .
Sc5 Pd1 Sc1 62.965(12) 9 9
Sc5 Pd1 Sc1 117.035(12) 10 9
Sc5 Pd1 Sc1 62.965(12) 2 9
Sc5 Pd1 Sc1 117.035(12) . 9
Sc5 Pd1 Sc1 62.965(12) 9 3
Sc5 Pd1 Sc1 117.035(12) 10 3
Sc5 Pd1 Sc1 62.965(12) 2 3
Sc5 Pd1 Sc1 117.035(12) . 3
Sc1 Pd1 Sc1 63.40(3) 9 3
Sc5 Pd1 Sc1 117.035(12) 9 11
Sc5 Pd1 Sc1 62.965(12) 10 11
Sc5 Pd1 Sc1 117.035(12) 2 11
Sc5 Pd1 Sc1 62.965(12) . 11
Sc1 Pd1 Sc1 116.60(3) 9 11
Sc1 Pd1 Sc1 180.00(3) 3 11
Sc5 Pd1 Sc1 117.035(12) 9 .
Sc5 Pd1 Sc1 62.965(12) 10 .
Sc5 Pd1 Sc1 117.035(12) 2 .
Sc5 Pd1 Sc1 62.965(12) . .
Sc1 Pd1 Sc1 180.0 9 .
Sc1 Pd1 Sc1 116.60(3) 3 .
Sc1 Pd1 Sc1 63.40(3) 11 .
Sc5 Pd1 Sc4 115.756(12) 9 .
Sc5 Pd1 Sc4 115.756(12) 10 .
Sc5 Pd1 Sc4 64.244(12) 2 .
Sc5 Pd1 Sc4 64.244(12) . .
Sc1 Pd1 Sc4 116.792(12) 9 .
Sc1 Pd1 Sc4 63.208(12) 3 .
Sc1 Pd1 Sc4 116.792(12) 11 .
Sc1 Pd1 Sc4 63.208(12) . .
Sc5 Pd1 Sc4 64.244(12) 9 9
Sc5 Pd1 Sc4 64.244(12) 10 9
Sc5 Pd1 Sc4 115.756(12) 2 9
Sc5 Pd1 Sc4 115.756(12) . 9
Sc1 Pd1 Sc4 63.208(12) 9 9
Sc1 Pd1 Sc4 116.792(12) 3 9
Sc1 Pd1 Sc4 63.208(12) 11 9
Sc1 Pd1 Sc4 116.792(12) . 9
Sc4 Pd1 Sc4 180.0 . 9
Sc5 Pd1 Sc4 64.244(12) 9 10
Sc5 Pd1 Sc4 64.244(12) 10 10
Sc5 Pd1 Sc4 115.756(12) 2 10
Sc5 Pd1 Sc4 115.756(12) . 10
Sc1 Pd1 Sc4 116.792(12) 9 10
Sc1 Pd1 Sc4 63.208(12) 3 10
Sc1 Pd1 Sc4 116.792(12) 11 10
Sc1 Pd1 Sc4 63.208(12) . 10
Sc4 Pd1 Sc4 61.87(3) . 10
Sc4 Pd1 Sc4 118.13(3) 9 10
Sc5 Pd1 Sc4 115.756(12) 9 2
Sc5 Pd1 Sc4 115.756(12) 10 2
Sc5 Pd1 Sc4 64.244(12) 2 2
Sc5 Pd1 Sc4 64.244(12) . 2
Sc1 Pd1 Sc4 63.208(12) 9 2
Sc1 Pd1 Sc4 116.792(12) 3 2
Sc1 Pd1 Sc4 63.208(12) 11 2
Sc1 Pd1 Sc4 116.792(12) . 2
Sc4 Pd1 Sc4 118.13(3) . 2
Sc4 Pd1 Sc4 61.87(3) 9 2
Sc4 Pd1 Sc4 180.00(3) 10 2
Sc9C Pd2 Sc1 145.9(5) . .
Sc9A Pd2 Sc1 138.5(4) . .
Sc1 Pd2 Sc9B 131.2(6) . .
Sc9C Pd2 Sc7 78.4(4) . 13
Sc9A Pd2 Sc7 84.6(4) . 13
Sc1 Pd2 Sc7 128.61(2) . 13
Sc9B Pd2 Sc7 90.8(5) . 13
Sc9C Pd2 Sc7 78.4(4) . 6_554
Sc9A Pd2 Sc7 84.6(4) . 6_554
Sc1 Pd2 Sc7 128.61(2) . 6_554
Sc9B Pd2 Sc7 90.8(5) . 6_554
Sc7 Pd2 Sc7 65.48(3) 13 6_554
Sc9C Pd2 Sc11 117.90(2) . 10
Sc9A Pd2 Sc11 117.916(18) . 10
Sc1 Pd2 Sc11 68.330(13) . 10
Sc9B Pd2 Sc11 117.44(6) . 10
Sc7 Pd2 Sc11 123.03(2) 13 10
Sc7 Pd2 Sc11 65.773(17) 6_554 10
Sc9C Pd2 Sc11 117.90(2) . .
Sc9A Pd2 Sc11 117.916(18) . .
Sc1 Pd2 Sc11 68.330(13) . .
Sc9B Pd2 Sc11 117.44(6) . .
Sc7 Pd2 Sc11 65.773(17) 13 .
Sc7 Pd2 Sc11 123.03(2) 6_554 .
Sc11 Pd2 Sc11 124.06(2) 10 .
Sc9C Pd2 Sc10 82.8(4) . 10
Sc9A Pd2 Sc10 76.6(3) . 10
Sc1 Pd2 Sc10 68.916(18) . 10
Sc9B Pd2 Sc10 70.6(5) . 10
Sc7 Pd2 Sc10 161.19(2) 13 10
Sc7 Pd2 Sc10 110.809(18) 6_554 10
Sc11 Pd2 Sc10 66.608(15) 10 10
Sc11 Pd2 Sc10 124.655(17) . 10
Sc9C Pd2 Sc10 82.8(4) . .
Sc9A Pd2 Sc10 76.6(3) . .
Sc1 Pd2 Sc10 68.916(18) . .
Sc9B Pd2 Sc10 70.6(5) . .
Sc7 Pd2 Sc10 110.810(17) 13 .
Sc7 Pd2 Sc10 161.19(2) 6_554 .
Sc11 Pd2 Sc10 124.654(17) 10 .
Sc11 Pd2 Sc10 66.610(15) . .
Sc10 Pd2 Sc10 66.28(2) 10 .
Sc9C Pd2 Sc3 143.8(5) . .
Sc9A Pd2 Sc3 151.2(4) . .
Sc1 Pd2 Sc3 70.30(3) . .
Sc9B Pd2 Sc3 158.5(6) . .
Sc7 Pd2 Sc3 71.30(2) 13 .
Sc7 Pd2 Sc3 71.30(2) 6_554 .
Sc11 Pd2 Sc3 66.627(13) 10 .
Sc11 Pd2 Sc3 66.627(13) . .
Sc10 Pd2 Sc3 126.201(19) 10 .
Sc10 Pd2 Sc3 126.202(19) . .
Sc4 Pd3 Sc7 121.87(3) . .
Sc4 Pd3 Sc12 124.29(2) . 13
Sc7 Pd3 Sc12 104.69(2) . 13
Sc4 Pd3 Sc12 124.29(2) . 14_455
Sc7 Pd3 Sc12 104.69(2) . 14_455
Sc12 Pd3 Sc12 61.51(3) 13 14_455
Sc4 Pd3 Sc6 66.951(17) . 12
Sc7 Pd3 Sc6 65.257(18) . 12
Sc12 Pd3 Sc6 168.70(2) 13 12
Sc12 Pd3 Sc6 114.593(18) 14_455 12
Sc4 Pd3 Sc6 66.952(17) . .
Sc7 Pd3 Sc6 65.256(18) . .
Sc12 Pd3 Sc6 114.593(18) 13 .
Sc12 Pd3 Sc6 168.70(2) 14_455 .
Sc6 Pd3 Sc6 66.99(2) 12 .
Sc4 Pd3 Pd5 176.48(2) . 13
Sc7 Pd3 Pd5 54.613(19) . 13
Sc12 Pd3 Pd5 58.501(18) 13 13
Sc12 Pd3 Pd5 58.501(18) 14_455 13
Sc6 Pd3 Pd5 110.221(14) 12 13
Sc6 Pd3 Pd5 110.220(14) . 13
Sc4 Pd3 Sc10 66.485(13) . .
Sc7 Pd3 Sc10 117.686(12) . .
Sc12 Pd3 Sc10 65.633(18) 13 .
Sc12 Pd3 Sc10 118.29(2) 14_455 .
Sc6 Pd3 Sc10 122.844(18) 12 .
Sc6 Pd3 Sc10 65.517(14) . .
Pd5 Pd3 Sc10 114.618(12) 13 .
Sc4 Pd3 Sc10 66.485(13) . 12
Sc7 Pd3 Sc10 117.685(12) . 12
Sc12 Pd3 Sc10 118.29(2) 13 12
Sc12 Pd3 Sc10 65.634(18) 14_455 12
Sc6 Pd3 Sc10 65.516(14) 12 12
Sc6 Pd3 Sc10 122.844(18) . 12
Pd5 Pd3 Sc10 114.619(12) 13 12
Sc10 Pd3 Sc10 120.18(2) . 12
Sc4 Pd3 Sc8 66.79(3) . .
Sc7 Pd3 Sc8 171.34(3) . .
Sc12 Pd3 Sc8 68.01(2) 13 .
Sc12 Pd3 Sc8 68.01(2) 14_455 .
Sc6 Pd3 Sc8 121.49(2) 12 .
Sc6 Pd3 Sc8 121.49(2) . .
Pd5 Pd3 Sc8 116.73(2) 13 .
Sc10 Pd3 Sc8 64.400(12) . .
Sc10 Pd3 Sc8 64.401(12) 12 .
Sc4 Pd3 Sc11 117.502(12) . 13
Sc7 Pd3 Sc11 61.219(11) . 13
Sc12 Pd3 Sc11 59.405(19) 13 13
Sc12 Pd3 Sc11 110.602(19) 14_455 13
Sc6 Pd3 Sc11 116.059(16) 12 13
Sc6 Pd3 Sc11 60.675(14) . 13
Pd5 Pd3 Sc11 61.441(10) 13 13
Sc10 Pd3 Sc11 62.504(14) . 13
Sc10 Pd3 Sc11 175.971(17) 12 13
Sc8 Pd3 Sc11 116.050(13) . 13
Sc4 Pd3 Sc11 117.502(12) . 8_455
Sc7 Pd3 Sc11 61.220(11) . 8_455
Sc12 Pd3 Sc11 110.602(19) 13 8_455
Sc12 Pd3 Sc11 59.405(19) 14_455 8_455
Sc6 Pd3 Sc11 60.676(14) 12 8_455
Sc6 Pd3 Sc11 116.059(16) . 8_455
Pd5 Pd3 Sc11 61.441(11) 13 8_455
Sc10 Pd3 Sc11 175.971(17) . 8_455
Sc10 Pd3 Sc11 62.503(14) 12 8_455
Sc8 Pd3 Sc11 116.050(13) . 8_455
Sc11 Pd3 Sc11 114.64(2) 13 8_455
Pd23 Pd4 Sc12 68.6(3) 13 .
Pd23 Pd4 Sc5 173.9(3) 13 .
Sc12 Pd4 Sc5 117.45(3) . .
Pd23 Pd4 Sc6 112.29(11) 13 11
Sc12 Pd4 Sc6 114.733(13) . 11
Sc5 Pd4 Sc6 65.860(12) . 11
Pd23 Pd4 Sc6 112.29(11) 13 .
Sc12 Pd4 Sc6 114.732(13) . .
Sc5 Pd4 Sc6 65.861(12) . .
Sc6 Pd4 Sc6 122.10(2) 11 .
Pd23 Pd4 Sc2 106.7(3) 13 .
Sc12 Pd4 Sc2 175.30(3) . .
Sc5 Pd4 Sc2 67.24(3) . .
Sc6 Pd4 Sc2 66.606(13) 11 .
Sc6 Pd4 Sc2 66.607(13) . .
Pd23 Pd4 Sc13 10.24(8) 13 13
Sc12 Pd4 Sc13 58.4(3) . 13
Sc5 Pd4 Sc13 175.8(3) . 13
Sc6 Pd4 Sc13 115.26(7) 11 13
Sc6 Pd4 Sc13 115.26(7) . 13
Sc2 Pd4 Sc13 116.9(3) . 13
Pd23 Pd4 Sc9B 51.9(5) 13 13
Sc12 Pd4 Sc9B 110.1(5) . 13
Sc5 Pd4 Sc9B 123.3(4) . 13
Sc6 Pd4 Sc9B 119.1(5) 11 13
Sc6 Pd4 Sc9B 67.3(4) . 13
Sc2 Pd4 Sc9B 66.0(5) . 13
Sc13 Pd4 Sc9B 60.1(5) 13 13
Pd23 Pd4 Sc9B 51.9(5) 13 7_545
Sc12 Pd4 Sc9B 110.1(5) . 7_545
Sc5 Pd4 Sc9B 123.3(4) . 7_545
Sc6 Pd4 Sc9B 67.3(4) 11 7_545
Sc6 Pd4 Sc9B 119.1(5) . 7_545
Sc2 Pd4 Sc9B 66.0(5) . 7_545
Sc13 Pd4 Sc9B 60.1(5) 13 7_545
Sc9B Pd4 Sc9B 59.7(9) 13 7_545
Pd23 Pd4 Sc11 120.2(3) 13 .
Sc12 Pd4 Sc11 62.743(19) . .
Sc5 Pd4 Sc11 64.711(17) . .
Sc6 Pd4 Sc11 118.261(17) 11 .
Sc6 Pd4 Sc11 63.860(14) . .
Sc2 Pd4 Sc11 121.02(2) . .
Sc13 Pd4 Sc11 111.9(2) 13 .
Sc9B Pd4 Sc11 118.0(5) 13 .
Sc9B Pd4 Sc11 171.9(5) 7_545 .
Pd23 Pd4 Sc11 120.2(3) 13 11
Sc12 Pd4 Sc11 62.743(19) . 11
Sc5 Pd4 Sc11 64.711(17) . 11
Sc6 Pd4 Sc11 63.859(14) 11 11
Sc6 Pd4 Sc11 118.261(17) . 11
Sc2 Pd4 Sc11 121.02(2) . 11
Sc13 Pd4 Sc11 111.9(2) 13 11
Sc9B Pd4 Sc11 171.9(5) 13 11
Sc9B Pd4 Sc11 118.0(5) 7_545 11
Sc11 Pd4 Sc11 62.97(2) . 11
Pd23 Pd4 Sc9A 57.3(4) 13 13
Sc12 Pd4 Sc9A 114.3(3) . 13
Sc5 Pd4 Sc9A 117.9(3) . 13
Sc6 Pd4 Sc9A 118.1(2) 11 13
Sc6 Pd4 Sc9A 63.0(2) . 13
Sc2 Pd4 Sc9A 61.9(3) . 13
Sc13 Pd4 Sc9A 65.4(3) 13 13
Sc11 Pd4 Sc9A 116.5(2) . 13
Sc11 Pd4 Sc9A 177.0(3) 11 13
Sc7 Pd5 Sc7 142.90(4) 14_545 13
Sc7 Pd5 Sc12 105.935(16) 14_545 2_655
Sc7 Pd5 Sc12 105.935(16) 13 2_655
Sc7 Pd5 Sc12 105.935(16) 14_545 .
Sc7 Pd5 Sc12 105.935(16) 13 .
Sc12 Pd5 Sc12 60.71(3) 2_655 .
Sc7 Pd5 Sc3 75.015(16) 14_545 .
Sc7 Pd5 Sc3 75.016(16) 13 .
Sc12 Pd5 Sc3 174.71(3) 2_655 .
Sc12 Pd5 Sc3 114.00(2) . .
Sc7 Pd5 Sc3 75.015(16) 14_545 9_655
Sc7 Pd5 Sc3 75.015(16) 13 9_655
Sc12 Pd5 Sc3 114.00(2) 2_655 9_655
Sc12 Pd5 Sc3 174.71(2) . 9_655
Sc3 Pd5 Sc3 71.29(3) . 9_655
Sc7 Pd5 Pd3 159.93(2) 14_545 13
Sc7 Pd5 Pd3 57.169(18) 13 13
Sc12 Pd5 Pd3 57.414(11) 2_655 13
Sc12 Pd5 Pd3 57.414(11) . 13
Sc3 Pd5 Pd3 120.477(9) . 13
Sc3 Pd5 Pd3 120.477(9) 9_655 13
Sc7 Pd5 Pd3 57.169(18) 14_545 14_545
Sc7 Pd5 Pd3 159.93(2) 13 14_545
Sc12 Pd5 Pd3 57.414(11) 2_655 14_545
Sc12 Pd5 Pd3 57.414(11) . 14_545
Sc3 Pd5 Pd3 120.477(9) . 14_545
Sc3 Pd5 Pd3 120.477(9) 9_655 14_545
Pd3 Pd5 Pd3 102.766(18) 13 14_545
Sc7 Pd5 Sc11 120.066(10) 14_545 .
Sc7 Pd5 Sc11 63.000(10) 13 .
Sc12 Pd5 Sc11 111.79(2) 2_655 .
Sc12 Pd5 Sc11 60.086(17) . .
Sc3 Pd5 Sc11 63.798(17) . .
Sc3 Pd5 Sc11 124.17(2) 9_655 .
Pd3 Pd5 Sc11 63.919(10) 13 .
Pd3 Pd5 Sc11 110.330(13) 14_545 .
Sc7 Pd5 Sc11 120.066(10) 14_545 12_655
Sc7 Pd5 Sc11 62.999(11) 13 12_655
Sc12 Pd5 Sc11 60.086(17) 2_655 12_655
Sc12 Pd5 Sc11 111.79(2) . 12_655
Sc3 Pd5 Sc11 124.17(2) . 12_655
Sc3 Pd5 Sc11 63.797(17) 9_655 12_655
Pd3 Pd5 Sc11 63.919(10) 13 12_655
Pd3 Pd5 Sc11 110.331(13) 14_545 12_655
Sc11 Pd5 Sc11 118.798(19) . 12_655
Sc7 Pd5 Sc11 62.999(11) 14_545 11
Sc7 Pd5 Sc11 120.066(10) 13 11
Sc12 Pd5 Sc11 111.79(2) 2_655 11
Sc12 Pd5 Sc11 60.087(17) . 11
Sc3 Pd5 Sc11 63.797(17) . 11
Sc3 Pd5 Sc11 124.17(2) 9_655 11
Pd3 Pd5 Sc11 110.331(13) 13 11
Pd3 Pd5 Sc11 63.919(10) 14_545 11
Sc11 Pd5 Sc11 60.486(19) . 11
Sc11 Pd5 Sc11 171.53(2) 12_655 11
Sc7 Pd5 Sc11 62.999(10) 14_545 2_655
Sc7 Pd5 Sc11 120.066(10) 13 2_655
Sc12 Pd5 Sc11 60.086(17) 2_655 2_655
Sc12 Pd5 Sc11 111.79(2) . 2_655
Sc3 Pd5 Sc11 124.17(2) . 2_655
Sc3 Pd5 Sc11 63.797(17) 9_655 2_655
Pd3 Pd5 Sc11 110.331(13) 13 2_655
Pd3 Pd5 Sc11 63.919(10) 14_545 2_655
Sc11 Pd5 Sc11 171.53(2) . 2_655
Sc11 Pd5 Sc11 60.487(19) 12_655 2_655
Sc11 Pd5 Sc11 118.798(19) 11 2_655
Pd2 Sc1 Pd1 179.89(3) . .
Pd2 Sc1 Sc5 122.327(19) . 10
Pd1 Sc1 Sc5 57.706(18) . 10
Pd2 Sc1 Sc5 122.327(19) . .
Pd1 Sc1 Sc5 57.707(18) . .
Sc5 Sc1 Sc5 106.69(3) 10 .
Pd2 Sc1 Sc1 121.809(17) . 11
Pd1 Sc1 Sc1 58.298(14) . 11
Sc5 Sc1 Sc1 59.507(14) 10 11
Sc5 Sc1 Sc1 59.507(14) . 11
Pd2 Sc1 Sc4 120.72(3) . .
Pd1 Sc1 Sc4 59.192(17) . .
Sc5 Sc1 Sc4 108.07(3) 10 .
Sc5 Sc1 Sc4 61.097(19) . .
Sc1 Sc1 Sc4 109.164(19) 11 .
Pd2 Sc1 Sc4 120.72(3) . 10
Pd1 Sc1 Sc4 59.193(17) . 10
Sc5 Sc1 Sc4 61.097(19) 10 10
Sc5 Sc1 Sc4 108.08(3) . 10
Sc1 Sc1 Sc4 109.164(19) 11 10
Sc4 Sc1 Sc4 59.29(3) . 10
Pd2 Sc1 Sc11 60.865(16) . 10
Pd1 Sc1 Sc11 119.169(17) . 10
Sc5 Sc1 Sc11 61.463(17) 10 10
Sc5 Sc1 Sc11 148.67(3) . 10
Sc1 Sc1 Sc11 91.470(17) 11 10
Sc4 Sc1 Sc11 148.25(3) . 10
Sc4 Sc1 Sc11 91.675(16) 10 10
Pd2 Sc1 Sc11 60.865(16) . .
Pd1 Sc1 Sc11 119.168(17) . .
Sc5 Sc1 Sc11 148.67(3) 10 .
Sc5 Sc1 Sc11 61.462(17) . .
Sc1 Sc1 Sc11 91.470(17) 11 .
Sc4 Sc1 Sc11 91.676(16) . .
Sc4 Sc1 Sc11 148.26(3) 10 .
Sc11 Sc1 Sc11 112.22(3) 10 .
Pd2 Sc1 Sc10 60.996(18) . 10
Pd1 Sc1 Sc10 118.92(2) . 10
Sc5 Sc1 Sc10 92.082(14) 10 10
Sc5 Sc1 Sc10 149.15(2) . 10
Sc1 Sc1 Sc10 149.078(12) 11 10
Sc4 Sc1 Sc10 90.16(2) . 10
Sc4 Sc1 Sc10 59.728(18) 10 10
Sc11 Sc1 Sc10 62.043(16) 10 10
Sc11 Sc1 Sc10 112.45(3) . 10
Pd2 Sc1 Sc10 60.996(18) . .
Pd1 Sc1 Sc10 118.92(2) . .
Sc5 Sc1 Sc10 149.15(2) 10 .
Sc5 Sc1 Sc10 92.082(14) . .
Sc1 Sc1 Sc10 149.079(12) 11 .
Sc4 Sc1 Sc10 59.728(18) . .
Sc4 Sc1 Sc10 90.16(2) 10 .
Sc11 Sc1 Sc10 112.45(3) 10 .
Sc11 Sc1 Sc10 62.045(16) . .
Sc10 Sc1 Sc10 61.65(2) 10 .
Pd2 Sc1 Sc3 60.453(18) . .
Pd1 Sc1 Sc3 119.65(3) . .
Sc5 Sc1 Sc3 91.88(2) 10 .
Sc5 Sc1 Sc3 91.88(2) . .
Sc1 Sc1 Sc3 61.356(16) 11 .
Sc4 Sc1 Sc3 149.725(15) . .
Sc4 Sc1 Sc3 149.725(15) 10 .
Sc11 Sc1 Sc3 61.540(15) 10 .
Sc11 Sc1 Sc3 61.540(15) . .
Sc10 Sc1 Sc3 112.18(2) 10 .
Sc10 Sc1 Sc3 112.18(2) . .
Pd4 Sc2 Pd4 168.37(4) . 2
Pd4 Sc2 Sc9C 70.1(4) . 13
Pd4 Sc2 Sc9C 118.7(4) 2 13
Pd4 Sc2 Sc9C 118.7(4) . 15_455
Pd4 Sc2 Sc9C 70.1(4) 2 15_455
Sc9C Sc2 Sc9C 48.7(8) 13 15_455
Pd4 Sc2 Sc9C 70.1(4) . 7_545
Pd4 Sc2 Sc9C 118.7(4) 2 7_545
Sc9C Sc2 Sc9C 73.2(9) 13 7_545
Sc9C Sc2 Sc9C 92.9(7) 15_455 7_545
Pd4 Sc2 Sc9C 118.7(4) . 5_445
Pd4 Sc2 Sc9C 70.1(4) 2 5_445
Sc9C Sc2 Sc9C 92.9(7) 13 5_445
Sc9C Sc2 Sc9C 73.2(9) 15_455 5_445
Sc9C Sc2 Sc9C 48.7(8) 7_545 5_445
Pd4 Sc2 Sc5 54.374(18) . .
Pd4 Sc2 Sc5 114.00(3) 2 .
Sc9C Sc2 Sc5 113.1(4) 13 .
Sc9C Sc2 Sc5 143.4(4) 15_455 .
Sc9C Sc2 Sc5 113.1(4) 7_545 .
Sc9C Sc2 Sc5 143.4(4) 5_445 .
Pd4 Sc2 Sc5 114.00(3) . 2
Pd4 Sc2 Sc5 54.375(18) 2 2
Sc9C Sc2 Sc5 143.4(4) 13 2
Sc9C Sc2 Sc5 113.1(4) 15_455 2
Sc9C Sc2 Sc5 143.4(4) 7_545 2
Sc9C Sc2 Sc5 113.1(4) 5_445 2
Sc5 Sc2 Sc5 59.62(3) . 2
Pd4 Sc2 Sc9A 64.6(3) . 13
Pd4 Sc2 Sc9A 124.4(3) 2 13
Sc5 Sc2 Sc9A 109.7(2) . 13
Sc5 Sc2 Sc9A 146.6(3) 2 13
Pd4 Sc2 Sc9A 124.4(3) . 15_455
Pd4 Sc2 Sc9A 64.6(3) 2 15_455
Sc5 Sc2 Sc9A 146.6(3) . 15_455
Sc5 Sc2 Sc9A 109.7(2) 2 15_455
Sc9A Sc2 Sc9A 60.0(6) 13 15_455
Pd4 Sc2 Sc9A 124.4(3) . 5_445
Pd4 Sc2 Sc9A 64.6(3) 2 5_445
Sc5 Sc2 Sc9A 146.6(3) . 5_445
Sc5 Sc2 Sc9A 109.7(2) 2 5_445
Sc9A Sc2 Sc9A 95.0(3) 13 5_445
Sc9A Sc2 Sc9A 65.6(6) 15_455 5_445
Pd4 Sc2 Sc9A 64.6(3) . 7_545
Pd4 Sc2 Sc9A 124.4(3) 2 7_545
Sc5 Sc2 Sc9A 109.7(2) . 7_545
Sc5 Sc2 Sc9A 146.6(3) 2 7_545
Sc9A Sc2 Sc9A 65.6(6) 13 7_545
Sc9A Sc2 Sc9A 95.0(3) 15_455 7_545
Sc9A Sc2 Sc9A 60.0(6) 5_445 7_545
Pd5 Sc3 Pd5 108.71(3) . 9_655
Pd5 Sc3 Pd2 97.022(9) . .
Pd5 Sc3 Pd2 97.022(9) 9_655 .
Pd5 Sc3 Pd2 97.022(9) . 11
Pd5 Sc3 Pd2 97.022(9) 9_655 11
Pd2 Sc3 Pd2 155.78(4) . 11
Pd5 Sc3 Sc1 120.758(13) . 11
Pd5 Sc3 Sc1 120.758(13) 9_655 11
Pd2 Sc3 Sc1 106.53(3) . 11
Pd2 Sc3 Sc1 49.247(18) 11 11
Pd5 Sc3 Sc1 120.758(13) . .
Pd5 Sc3 Sc1 120.758(13) 9_655 .
Pd2 Sc3 Sc1 49.246(18) . .
Pd2 Sc3 Sc1 106.53(3) 11 .
Sc1 Sc3 Sc1 57.29(3) 11 .
Pd5 Sc3 Sc11 147.602(19) . 4
Pd5 Sc3 Sc11 63.251(11) 9_655 4
Pd2 Sc3 Sc11 114.781(19) . 4
Pd2 Sc3 Sc11 55.868(11) 11 4
Sc1 Sc3 Sc11 57.507(16) 11 4
Sc1 Sc3 Sc11 86.76(2) . 4
Pd5 Sc3 Sc11 147.602(19) . 10
Pd5 Sc3 Sc11 63.251(11) 9_655 10
Pd2 Sc3 Sc11 55.868(11) . 10
Pd2 Sc3 Sc11 114.782(19) 11 10
Sc1 Sc3 Sc11 86.76(2) 11 10
Sc1 Sc3 Sc11 57.507(16) . 10
Sc11 Sc3 Sc11 60.17(2) 4 10
Pd5 Sc3 Sc11 63.251(11) . 11
Pd5 Sc3 Sc11 147.602(19) 9_655 11
Pd2 Sc3 Sc11 114.781(19) . 11
Pd2 Sc3 Sc11 55.868(11) 11 11
Sc1 Sc3 Sc11 57.507(16) 11 11
Sc1 Sc3 Sc11 86.76(2) . 11
Sc11 Sc3 Sc11 105.58(3) 4 11
Sc11 Sc3 Sc11 140.45(4) 10 11
Pd5 Sc3 Sc11 63.251(11) . .
Pd5 Sc3 Sc11 147.603(19) 9_655 .
Pd2 Sc3 Sc11 55.869(11) . .
Pd2 Sc3 Sc11 114.781(19) 11 .
Sc1 Sc3 Sc11 86.76(2) 11 .
Sc1 Sc3 Sc11 57.508(16) . .
Sc11 Sc3 Sc11 140.45(4) 4 .
Sc11 Sc3 Sc11 105.58(3) 10 .
Sc11 Sc3 Sc11 60.17(2) 11 .
Pd5 Sc3 Sc3 54.357(17) . 9_655
Pd5 Sc3 Sc3 54.357(17) 9_655 9_655
Pd2 Sc3 Sc3 102.11(2) . 9_655
Pd2 Sc3 Sc3 102.11(2) 11 9_655
Sc1 Sc3 Sc3 151.357(16) 11 9_655
Sc1 Sc3 Sc3 151.356(16) . 9_655
Sc11 Sc3 Sc3 109.773(19) 4 9_655
Sc11 Sc3 Sc3 109.773(19) 10 9_655
Sc11 Sc3 Sc3 109.773(19) 11 9_655
Sc11 Sc3 Sc3 109.773(19) . 9_655
Pd5 Sc3 Sc7 49.064(16) . 13
Pd5 Sc3 Sc7 94.18(2) 9_655 13
Pd2 Sc3 Sc7 51.679(12) . 13
Pd2 Sc3 Sc7 146.07(2) 11 13
Sc1 Sc3 Sc7 142.55(2) 11 13
Sc1 Sc3 Sc7 94.767(16) . 13
Sc11 Sc3 Sc7 153.83(2) 4 13
Sc11 Sc3 Sc7 98.868(17) 10 13
Sc11 Sc3 Sc7 100.597(16) 11 13
Sc11 Sc3 Sc7 55.986(13) . 13
Sc3 Sc3 Sc7 60.024(17) 9_655 13
Pd3 Sc4 Pd1 175.83(3) . .
Pd3 Sc4 Sc4 125.102(17) . 10
Pd1 Sc4 Sc4 59.067(14) . 10
Pd3 Sc4 Sc6 61.758(18) . 12
Pd1 Sc4 Sc6 114.88(2) . 12
Sc4 Sc4 Sc6 148.084(12) 10 12
Pd3 Sc4 Sc6 61.758(18) . .
Pd1 Sc4 Sc6 114.88(2) . .
Sc4 Sc4 Sc6 148.084(12) 10 .
Sc6 Sc4 Sc6 63.79(2) 12 .
Pd3 Sc4 Sc1 123.572(18) . 3
Pd1 Sc4 Sc1 57.600(17) . 3
Sc4 Sc4 Sc1 60.357(13) 10 3
Sc6 Sc4 Sc1 89.350(14) 12 3
Sc6 Sc4 Sc1 147.04(3) . 3
Pd3 Sc4 Sc1 123.572(18) . .
Pd1 Sc4 Sc1 57.600(17) . .
Sc4 Sc4 Sc1 60.357(13) 10 .
Sc6 Sc4 Sc1 147.04(3) 12 .
Sc6 Sc4 Sc1 89.350(14) . .
Sc1 Sc4 Sc1 107.17(3) 3 .
Pd3 Sc4 Sc10 62.819(16) . .
Pd1 Sc4 Sc10 118.469(16) . .
Sc4 Sc4 Sc10 91.452(16) 10 .
Sc6 Sc4 Sc10 115.64(2) 12 .
Sc6 Sc4 Sc10 62.872(15) . .
Sc1 Sc4 Sc10 150.08(3) 3 .
Sc1 Sc4 Sc10 60.872(17) . .
Pd3 Sc4 Sc10 62.820(16) . 12
Pd1 Sc4 Sc10 118.468(16) . 12
Sc4 Sc4 Sc10 91.452(16) 10 12
Sc6 Sc4 Sc10 62.872(15) 12 12
Sc6 Sc4 Sc10 115.64(2) . 12
Sc1 Sc4 Sc10 60.872(17) 3 12
Sc1 Sc4 Sc10 150.08(3) . 12
Sc10 Sc4 Sc10 114.48(3) . 12
Pd3 Sc4 Sc5 120.30(2) . 2
Pd1 Sc4 Sc5 56.307(17) . 2
Sc4 Sc4 Sc5 106.822(18) 10 2
Sc6 Sc4 Sc5 58.576(18) 12 2
Sc6 Sc4 Sc5 90.01(2) . 2
Sc1 Sc4 Sc5 58.448(19) 3 2
Sc1 Sc4 Sc5 105.73(3) . 2
Sc10 Sc4 Sc5 148.32(2) . 2
Sc10 Sc4 Sc5 91.200(16) 12 2
Pd3 Sc4 Sc5 120.30(2) . .
Pd1 Sc4 Sc5 56.308(17) . .
Sc4 Sc4 Sc5 106.823(18) 10 .
Sc6 Sc4 Sc5 90.01(2) 12 .
Sc6 Sc4 Sc5 58.575(18) . .
Sc1 Sc4 Sc5 105.73(3) 3 .
Sc1 Sc4 Sc5 58.448(19) . .
Sc10 Sc4 Sc5 91.201(16) . .
Sc10 Sc4 Sc5 148.32(2) 12 .
Sc5 Sc4 Sc5 59.15(3) 2 .
Pd3 Sc4 Sc8 63.91(2) . .
Pd1 Sc4 Sc8 120.26(2) . .
Sc4 Sc4 Sc8 61.192(16) 10 .
Sc6 Sc4 Sc8 115.15(2) 12 .
Sc6 Sc4 Sc8 115.15(2) . .
Sc1 Sc4 Sc8 92.83(2) 3 .
Sc1 Sc4 Sc8 92.83(2) . .
Sc10 Sc4 Sc8 62.520(16) . .
Sc10 Sc4 Sc8 62.522(16) 12 .
Sc5 Sc4 Sc8 149.105(15) 2 .
Sc5 Sc4 Sc8 149.106(15) . .
Pd4 Sc5 Pd1 176.28(3) . .
Pd4 Sc5 Sc1 123.65(2) . 11
Pd1 Sc5 Sc1 59.328(17) . 11
Pd4 Sc5 Sc1 123.65(2) . .
Pd1 Sc5 Sc1 59.328(17) . .
Sc1 Sc5 Sc1 60.99(3) 11 .
Pd4 Sc5 Sc6 59.122(15) . 11
Pd1 Sc5 Sc6 119.756(17) . 11
Sc1 Sc5 Sc6 91.578(16) 11 11
Sc1 Sc5 Sc6 149.62(3) . 11
Pd4 Sc5 Sc6 59.121(15) . .
Pd1 Sc5 Sc6 119.757(17) . .
Sc1 Sc5 Sc6 149.62(3) 11 .
Sc1 Sc5 Sc6 91.578(17) . .
Sc6 Sc5 Sc6 110.77(3) 11 .
Pd4 Sc5 Sc5 118.572(16) . 2
Pd1 Sc5 Sc5 57.706(14) . 2
Sc1 Sc5 Sc5 108.331(19) 11 2
Sc1 Sc5 Sc5 108.331(19) . 2
Sc6 Sc5 Sc5 91.806(16) 11 2
Sc6 Sc5 Sc5 91.806(16) . 2
Pd4 Sc5 Sc2 58.383(18) . .
Pd1 Sc5 Sc2 117.89(3) . .
Sc1 Sc5 Sc2 148.478(16) 11 .
Sc1 Sc5 Sc2 148.478(16) . .
Sc6 Sc5 Sc2 61.544(15) 11 .
Sc6 Sc5 Sc2 61.544(15) . .
Sc5 Sc5 Sc2 60.189(16) 2 .
Pd4 Sc5 Sc4 119.354(18) . .
Pd1 Sc5 Sc4 59.448(17) . .
Sc1 Sc5 Sc4 109.83(3) 11 .
Sc1 Sc5 Sc4 60.455(19) . .
Sc6 Sc5 Sc4 148.72(3) 11 .
Sc6 Sc5 Sc4 60.314(16) . .
Sc5 Sc5 Sc4 60.426(13) 2 .
Sc2 Sc5 Sc4 90.329(19) . .
Pd4 Sc5 Sc4 119.353(18) . 2
Pd1 Sc5 Sc4 59.449(17) . 2
Sc1 Sc5 Sc4 60.455(19) 11 2
Sc1 Sc5 Sc4 109.83(3) . 2
Sc6 Sc5 Sc4 60.312(16) 11 2
Sc6 Sc5 Sc4 148.72(3) . 2
Sc5 Sc5 Sc4 60.426(13) 2 2
Sc2 Sc5 Sc4 90.328(19) . 2
Sc4 Sc5 Sc4 110.20(3) . 2
Pd4 Sc5 Sc11 63.404(18) . .
Pd1 Sc5 Sc11 119.61(2) . .
Sc1 Sc5 Sc11 91.64(2) 11 .
Sc1 Sc5 Sc11 60.286(18) . .
Sc6 Sc5 Sc11 111.91(3) 11 .
Sc6 Sc5 Sc11 61.506(16) . .
Sc5 Sc5 Sc11 148.774(12) 2 .
Sc2 Sc5 Sc11 112.76(2) . .
Sc4 Sc5 Sc11 90.640(14) . .
Sc4 Sc5 Sc11 149.14(2) 2 .
Pd4 Sc5 Sc11 63.405(18) . 11
Pd1 Sc5 Sc11 119.61(2) . 11
Sc1 Sc5 Sc11 60.285(18) 11 11
Sc1 Sc5 Sc11 91.64(2) . 11
Sc6 Sc5 Sc11 61.507(16) 11 11
Sc6 Sc5 Sc11 111.91(3) . 11
Sc5 Sc5 Sc11 148.773(12) 2 11
Sc2 Sc5 Sc11 112.76(2) . 11
Sc4 Sc5 Sc11 149.14(2) . 11
Sc4 Sc5 Sc11 90.638(14) 2 11
Sc11 Sc5 Sc11 62.20(2) . 11
Pd4 Sc6 Pd3 166.66(2) . .
Pd4 Sc6 Sc5 55.018(16) . .
Pd3 Sc6 Sc5 112.38(2) . .
Pd4 Sc6 Sc7 133.67(2) . .
Pd3 Sc6 Sc7 53.270(18) . .
Sc5 Sc6 Sc7 145.80(2) . .
Pd4 Sc6 Sc4 116.05(2) . .
Pd3 Sc6 Sc4 51.290(16) . .
Sc5 Sc6 Sc4 61.11(2) . .
Sc7 Sc6 Sc4 98.27(2) . .
Pd4 Sc6 Sc10 66.526(16) . 13
Pd3 Sc6 Sc10 126.21(2) . 13
Sc5 Sc6 Sc10 111.92(2) . 13
Sc7 Sc6 Sc10 99.284(19) . 13
Sc4 Sc6 Sc10 149.47(2) . 13
Pd4 Sc6 Sc2 56.702(12) . .
Pd3 Sc6 Sc2 114.883(17) . .
Sc5 Sc6 Sc2 60.11(2) . .
Sc7 Sc6 Sc2 95.59(2) . .
Sc4 Sc6 Sc2 89.97(2) . .
Sc10 Sc6 Sc2 112.86(2) 13 .
Pd4 Sc6 Sc11 61.812(15) . .
Pd3 Sc6 Sc11 118.03(2) . .
Sc5 Sc6 Sc11 60.754(19) . .
Sc7 Sc6 Sc11 152.01(2) . .
Sc4 Sc6 Sc11 90.661(18) . .
Sc10 Sc6 Sc11 62.936(17) 13 .
Sc2 Sc6 Sc11 110.97(2) . .
Pd4 Sc6 Sc11 128.03(2) . 13
Pd3 Sc6 Sc11 64.763(15) . 13
Sc5 Sc6 Sc11 149.25(2) . 13
Sc7 Sc6 Sc11 59.462(17) . 13
Sc4 Sc6 Sc11 107.96(2) . 13
Sc10 Sc6 Sc11 61.517(17) 13 13
Sc2 Sc6 Sc11 150.46(3) . 13
Sc11 Sc6 Sc11 92.555(19) . 13
Pd4 Sc6 Sc9C 68.7(5) . 13
Pd3 Sc6 Sc9C 117.3(5) . 13
Sc5 Sc6 Sc9C 112.0(5) . 13
Sc7 Sc6 Sc9C 65.0(5) . 13
Sc4 Sc6 Sc9C 140.1(4) . 13
Sc10 Sc6 Sc9C 70.4(4) 13 13
Sc2 Sc6 Sc9C 58.3(5) . 13
Sc11 Sc6 Sc9C 121.6(4) . 13
Sc11 Sc6 Sc9C 94.5(5) 13 13
Pd4 Sc6 Sc9A 64.0(3) . 13
Pd3 Sc6 Sc9A 122.7(3) . 13
Sc5 Sc6 Sc9A 110.0(3) . 13
Sc7 Sc6 Sc9A 70.0(3) . 13
Sc4 Sc6 Sc9A 144.6(3) . 13
Sc10 Sc6 Sc9A 65.6(3) 13 13
Sc2 Sc6 Sc9A 59.5(2) . 13
Sc11 Sc6 Sc9A 115.7(3) . 13
Sc11 Sc6 Sc9A 94.8(2) 13 13
Pd4 Sc6 Sc10 121.80(2) . .
Pd3 Sc6 Sc10 58.049(14) . .
Sc5 Sc6 Sc10 90.27(2) . .
Sc7 Sc6 Sc10 102.04(2) . .
Sc4 Sc6 Sc10 58.794(16) . .
Sc10 Sc6 Sc10 93.091(19) 13 .
Sc2 Sc6 Sc10 145.78(3) . .
Sc11 Sc6 Sc10 60.437(16) . .
Sc11 Sc6 Sc10 61.582(17) 13 .
Sc9C Sc6 Sc10 155.8(5) 13 .
Sc9A Sc6 Sc10 154.6(2) 13 .
Pd5 Sc7 Pd3 68.22(2) 13 .
Pd5 Sc7 Pd2 108.34(2) 13 13
Pd3 Sc7 Pd2 123.262(14) . 13
Pd5 Sc7 Pd2 108.34(2) 13 15_455
Pd3 Sc7 Pd2 123.262(14) . 15_455
Pd2 Sc7 Pd2 111.70(3) 13 15_455
Pd5 Sc7 Sc7 108.554(19) 13 10_556
Pd3 Sc7 Sc7 176.770(18) . 10_556
Pd2 Sc7 Sc7 57.259(14) 13 10_556
Pd2 Sc7 Sc7 57.259(13) 15_455 10_556
Pd5 Sc7 Sc6 118.08(3) 13 .
Pd3 Sc7 Sc6 61.474(18) . .
Pd2 Sc7 Sc6 74.726(15) 13 .
Pd2 Sc7 Sc6 128.33(3) 15_455 .
Sc7 Sc7 Sc6 121.073(17) 10_556 .
Pd5 Sc7 Sc6 118.08(3) 13 12
Pd3 Sc7 Sc6 61.473(18) . 12
Pd2 Sc7 Sc6 128.33(3) 13 12
Pd2 Sc7 Sc6 74.727(15) 15_455 12
Sc7 Sc7 Sc6 121.073(17) 10_556 12
Sc6 Sc7 Sc6 64.54(2) . 12
Pd5 Sc7 Sc11 67.934(17) 13 8_455
Pd3 Sc7 Sc11 68.787(17) . 8_455
Pd2 Sc7 Sc11 166.04(3) 13 8_455
Pd2 Sc7 Sc11 59.248(11) 15_455 8_455
Sc7 Sc7 Sc11 110.280(16) 10_556 8_455
Sc6 Sc7 Sc11 119.12(3) . 8_455
Sc6 Sc7 Sc11 62.006(16) 12 8_455
Pd5 Sc7 Sc11 67.934(17) 13 13
Pd3 Sc7 Sc11 68.787(17) . 13
Pd2 Sc7 Sc11 59.248(11) 13 13
Pd2 Sc7 Sc11 166.04(3) 15_455 13
Sc7 Sc7 Sc11 110.280(17) 10_556 13
Sc6 Sc7 Sc11 62.005(16) . 13
Sc6 Sc7 Sc11 119.11(3) 12 13
Sc11 Sc7 Sc11 127.08(3) 8_455 13
Pd5 Sc7 Sc9C 155.6(4) 13 15_455
Pd3 Sc7 Sc9C 119.5(2) . 15_455
Pd2 Sc7 Sc9C 87.1(3) 13 15_455
Pd2 Sc7 Sc9C 47.4(4) 15_455 15_455
Sc7 Sc7 Sc9C 63.4(2) 10_556 15_455
Sc6 Sc7 Sc9C 83.7(4) . 15_455
Sc6 Sc7 Sc9C 59.1(2) 12 15_455
Sc11 Sc7 Sc9C 92.5(4) 8_455 15_455
Sc11 Sc7 Sc9C 136.1(4) 13 15_455
Pd5 Sc7 Sc9C 155.6(4) 13 13
Pd3 Sc7 Sc9C 119.5(2) . 13
Pd2 Sc7 Sc9C 47.4(4) 13 13
Pd2 Sc7 Sc9C 87.1(3) 15_455 13
Sc7 Sc7 Sc9C 63.4(2) 10_556 13
Sc6 Sc7 Sc9C 59.1(2) . 13
Sc6 Sc7 Sc9C 83.7(4) 12 13
Sc11 Sc7 Sc9C 136.1(4) 8_455 13
Sc11 Sc7 Sc9C 92.5(4) 13 13
Sc9C Sc7 Sc9C 44.4(8) 15_455 13
Pd5 Sc7 Sc3 55.921(17) 13 13
Pd3 Sc7 Sc3 113.92(2) . 13
Pd2 Sc7 Sc3 57.025(17) 13 13
Pd2 Sc7 Sc3 106.42(3) 15_455 13
Sc7 Sc7 Sc3 63.387(14) 10_556 13
Sc6 Sc7 Sc3 117.451(18) . 13
Sc6 Sc7 Sc3 174.00(3) 12 13
Sc11 Sc7 Sc3 113.27(3) 8_455 13
Sc11 Sc7 Sc3 60.027(19) 13 13
Sc9C Sc7 Sc3 126.1(2) 15_455 13
Sc9C Sc7 Sc3 102.2(4) 13 13
Sc13 Sc8 Sc13 113.8(3) 9_565 .
Sc13 Sc8 Pd3 96.46(3) 9_565 .
Sc13 Sc8 Pd3 96.46(3) . .
Sc13 Sc8 Pd3 96.46(3) 9_565 10
Sc13 Sc8 Pd3 96.46(3) . 10
Pd3 Sc8 Pd3 156.22(4) . 10
Sc13 Sc8 Sc4 118.60(13) 9_565 10
Sc13 Sc8 Sc4 118.60(13) . 10
Pd3 Sc8 Sc4 106.92(3) . 10
Pd3 Sc8 Sc4 49.299(17) 10 10
Sc13 Sc8 Sc4 118.60(13) 9_565 .
Sc13 Sc8 Sc4 118.60(13) . .
Pd3 Sc8 Sc4 49.301(17) . .
Pd3 Sc8 Sc4 106.91(3) 10 .
Sc4 Sc8 Sc4 57.62(3) 10 .
Sc13 Sc8 Sc10 148.87(5) 9_565 .
Sc13 Sc8 Sc10 60.94(13) . .
Pd3 Sc8 Sc10 56.436(11) . .
Pd3 Sc8 Sc10 114.405(19) 10 .
Sc4 Sc8 Sc10 86.61(3) 10 .
Sc4 Sc8 Sc10 57.668(17) . .
Sc13 Sc8 Sc10 60.94(13) 9_565 3
Sc13 Sc8 Sc10 148.87(5) . 3
Pd3 Sc8 Sc10 114.405(19) . 3
Pd3 Sc8 Sc10 56.436(11) 10 3
Sc4 Sc8 Sc10 57.667(17) 10 3
Sc4 Sc8 Sc10 86.61(3) . 3
Sc10 Sc8 Sc10 140.38(4) . 3
Sc13 Sc8 Sc10 60.94(13) 9_565 12
Sc13 Sc8 Sc10 148.87(5) . 12
Pd3 Sc8 Sc10 56.436(11) . 12
Pd3 Sc8 Sc10 114.405(19) 10 12
Sc4 Sc8 Sc10 86.61(3) 10 12
Sc4 Sc8 Sc10 57.667(17) . 12
Sc10 Sc8 Sc10 106.44(3) . 12
Sc10 Sc8 Sc10 59.16(2) 3 12
Sc13 Sc8 Sc10 148.87(5) 9_565 10
Sc13 Sc8 Sc10 60.94(13) . 10
Pd3 Sc8 Sc10 114.405(19) . 10
Pd3 Sc8 Sc10 56.436(11) 10 10
Sc4 Sc8 Sc10 57.667(16) 10 10
Sc4 Sc8 Sc10 86.61(3) . 10
Sc10 Sc8 Sc10 59.16(2) . 10
Sc10 Sc8 Sc10 106.44(3) 3 10
Sc10 Sc8 Sc10 140.38(4) 12 10
Sc13 Sc8 Sc12 94.74(11) 9_565 13
Sc13 Sc8 Sc12 50.15(4) . 13
Pd3 Sc8 Sc12 51.531(13) . 13
Pd3 Sc8 Sc12 146.37(2) 10 13
Sc4 Sc8 Sc12 143.69(2) 10 13
Sc4 Sc8 Sc12 95.135(16) . 13
Sc10 Sc8 Sc12 57.344(14) . 13
Sc10 Sc8 Sc12 152.36(2) 3 13
Sc10 Sc8 Sc12 98.747(18) 12 13
Sc10 Sc8 Sc12 101.201(17) 10 13
Sc13 Sc8 Sc12 50.15(4) 9_565 14_455
Sc13 Sc8 Sc12 94.74(11) . 14_455
Pd3 Sc8 Sc12 51.531(13) . 14_455
Pd3 Sc8 Sc12 146.37(2) 10 14_455
Sc4 Sc8 Sc12 143.69(2) 10 14_455
Sc4 Sc8 Sc12 95.135(16) . 14_455
Sc10 Sc8 Sc12 98.747(18) . 14_455
Sc10 Sc8 Sc12 101.201(17) 3 14_455
Sc10 Sc8 Sc12 57.345(14) 12 14_455
Sc10 Sc8 Sc12 152.36(2) 10 14_455
Sc12 Sc8 Sc12 51.16(3) 13 14_455
Pd2 Sc9A Pd23 110.1(6) . .
Pd2 Sc9A Sc9A 106.7(4) . 3_655
Pd23 Sc9A Sc9A 143.2(3) . 3_655
Pd2 Sc9A Sc2 131.5(4) . 13
Pd23 Sc9A Sc2 94.3(4) . 13
Sc9A Sc9A Sc2 60.0(3) 3_655 13
Pd2 Sc9A Sc2 131.5(4) . 5_554
Pd23 Sc9A Sc2 94.3(4) . 5_554
Sc9A Sc9A Sc2 60.0(3) 3_655 5_554
Sc2 Sc9A Sc2 85.0(3) 13 5_554
Pd2 Sc9A Sc6 75.7(3) . 6_554
Pd23 Sc9A Sc6 97.7(3) . 6_554
Sc9A Sc9A Sc6 91.2(3) 3_655 6_554
Sc2 Sc9A Sc6 143.2(4) 13 6_554
Sc2 Sc9A Sc6 59.53(8) 5_554 6_554
Pd2 Sc9A Sc6 75.7(3) . 13
Pd23 Sc9A Sc6 97.7(3) . 13
Sc9A Sc9A Sc6 91.2(3) 3_655 13
Sc2 Sc9A Sc6 59.53(8) 13 13
Sc2 Sc9A Sc6 143.2(4) 5_554 13
Sc6 Sc9A Sc6 150.8(5) 6_554 13
Pd2 Sc9A Pd4 113.1(4) . 13
Pd23 Sc9A Pd4 50.6(3) . 13
Sc9A Sc9A Pd4 113.4(3) 3_655 13
Sc2 Sc9A Pd4 53.48(15) 13 13
Sc2 Sc9A Pd4 114.7(5) 5_554 13
Sc6 Sc9A Pd4 148.2(6) 6_554 13
Sc6 Sc9A Pd4 53.06(9) 13 13
Pd2 Sc9A Pd4 113.1(4) . 6_554
Pd23 Sc9A Pd4 50.6(3) . 6_554
Sc9A Sc9A Pd4 113.4(3) 3_655 6_554
Sc2 Sc9A Pd4 114.7(5) 13 6_554
Sc2 Sc9A Pd4 53.48(15) 5_554 6_554
Sc6 Sc9A Pd4 53.06(9) 6_554 6_554
Sc6 Sc9A Pd4 148.2(6) 13 6_554
Pd4 Sc9A Pd4 97.1(5) 13 6_554
Pd2 Sc9A Sc13 104.3(5) . .
Pd23 Sc9A Sc13 5.75(8) . .
Sc9A Sc9A Sc13 149.0(3) 3_655 .
Sc2 Sc9A Sc13 98.5(4) 13 .
Sc2 Sc9A Sc13 98.5(4) 5_554 .
Sc6 Sc9A Sc13 96.4(3) 6_554 .
Sc6 Sc9A Sc13 96.4(3) 13 .
Pd4 Sc9A Sc13 52.2(3) 13 .
Pd4 Sc9A Sc13 52.2(3) 6_554 .
Pd2 Sc9A Sc9A 163.3(4) . 11_565
Pd23 Sc9A Sc9A 53.2(3) . 11_565
Sc9A Sc9A Sc9A 90.0 3_655 11_565
Sc2 Sc9A Sc9A 57.2(3) 13 11_565
Sc2 Sc9A Sc9A 57.2(3) 5_554 11_565
Sc6 Sc9A Sc9A 104.6(3) 6_554 11_565
Sc6 Sc9A Sc9A 104.6(3) 13 11_565
Pd4 Sc9A Sc9A 58.0(2) 13 11_565
Pd4 Sc9A Sc9A 58.0(2) 6_554 11_565
Sc13 Sc9A Sc9A 59.0(3) . 11_565
Pd2 Sc9A Sc10 57.1(3) . 10
Pd23 Sc9A Sc10 62.3(4) . 10
Sc9A Sc9A Sc10 145.2(2) 3_655 10
Sc2 Sc9A Sc10 154.6(6) 13 10
Sc2 Sc9A Sc10 105.42(18) 5_554 10
Sc6 Sc9A Sc10 56.33(15) 6_554 10
Sc6 Sc9A Sc10 111.0(4) 13 10
Pd4 Sc9A Sc10 101.4(5) 13 10
Pd4 Sc9A Sc10 59.4(2) 6_554 10
Sc13 Sc9A Sc10 57.5(3) . 10
Sc9A Sc9A Sc10 108.7(3) 11_565 10
Pd23 Sc9B Pd2 117.7(11) . .
Pd23 Sc9B Sc13 6.49(15) . .
Pd2 Sc9B Sc13 111.2(10) . .
Pd23 Sc9B Sc9B 53.0(7) . 11_565
Pd2 Sc9B Sc9B 170.6(6) . 11_565
Sc13 Sc9B Sc9B 59.4(6) . 11_565
Pd23 Sc9B Pd4 55.8(4) . 13
Pd2 Sc9B Pd4 116.0(6) . 13
Sc13 Sc9B Pd4 57.6(4) . 13
Sc9B Sc9B Pd4 60.1(4) 11_565 13
Pd23 Sc9B Pd4 55.8(4) . 6_554
Pd2 Sc9B Pd4 116.0(6) . 6_554
Sc13 Sc9B Pd4 57.6(4) . 6_554
Sc9B Sc9B Pd4 60.1(4) 11_565 6_554
Pd4 Sc9B Pd4 106.8(7) 13 6_554
Pd23 Sc9B Sc2 100.6(6) . 13
Pd2 Sc9B Sc2 123.9(6) . 13
Sc13 Sc9B Sc2 105.3(6) . 13
Sc9B Sc9B Sc2 62.1(4) 11_565 13
Pd4 Sc9B Sc2 54.9(3) 13 13
Pd4 Sc9B Sc2 119.4(8) 6_554 13
Pd23 Sc9B Sc2 100.6(6) . 5_554
Pd2 Sc9B Sc2 123.9(6) . 5_554
Sc13 Sc9B Sc2 105.3(6) . 5_554
Sc9B Sc9B Sc2 62.1(4) 11_565 5_554
Pd4 Sc9B Sc2 119.4(8) 13 5_554
Pd4 Sc9B Sc2 54.9(3) 6_554 5_554
Sc2 Sc9B Sc2 83.2(7) 13 5_554
Pd23 Sc9B Sc6 104.0(5) . 6_554
Pd2 Sc9B Sc6 72.9(4) . 6_554
Sc13 Sc9B Sc6 102.6(5) . 6_554
Sc9B Sc9B Sc6 108.0(4) 11_565 6_554
Pd4 Sc9B Sc6 159.8(8) 13 6_554
Pd4 Sc9B Sc6 54.24(5) 6_554 6_554
Sc2 Sc9B Sc6 137.2(9) 13 6_554
Sc2 Sc9B Sc6 58.31(19) 5_554 6_554
Pd23 Sc9B Sc6 104.0(5) . 13
Pd2 Sc9B Sc6 72.9(4) . 13
Sc13 Sc9B Sc6 102.6(5) . 13
Sc9B Sc9B Sc6 108.0(4) 11_565 13
Pd4 Sc9B Sc6 54.24(5) 13 13
Pd4 Sc9B Sc6 159.8(8) 6_554 13
Sc2 Sc9B Sc6 58.31(19) 13 13
Sc2 Sc9B Sc6 137.2(9) 5_554 13
Sc6 Sc9B Sc6 143.0(8) 6_554 13
Pd23 Sc9B Sc10 68.0(6) . 10
Pd2 Sc9B Sc10 58.6(5) . 10
Sc13 Sc9B Sc10 62.6(5) . 10
Sc9B Sc9B Sc10 113.6(4) 11_565 10
Pd4 Sc9B Sc10 110.1(8) 13 10
Pd4 Sc9B Sc10 63.2(4) 6_554 10
Sc2 Sc9B Sc10 164.9(7) 13 10
Sc2 Sc9B Sc10 107.98(14) 5_554 10
Sc6 Sc9B Sc10 57.4(3) 6_554 10
Sc6 Sc9B Sc10 113.5(8) 13 10
Pd23 Sc9B Sc10 68.0(6) . .
Pd2 Sc9B Sc10 58.6(5) . .
Sc13 Sc9B Sc10 62.6(5) . .
Sc9B Sc9B Sc10 113.6(4) 11_565 .
Pd4 Sc9B Sc10 63.2(4) 13 .
Pd4 Sc9B Sc10 110.1(8) 6_554 .
Sc2 Sc9B Sc10 107.98(14) 13 .
Sc2 Sc9B Sc10 164.9(7) 5_554 .
Sc6 Sc9B Sc10 113.5(8) 6_554 .
Sc6 Sc9B Sc10 57.4(3) 13 .
Sc10 Sc9B Sc10 59.3(5) 10 .
Pd2 Sc9C Sc9C 114.1(5) . 3_655
Pd2 Sc9C Sc2 135.5(4) . 13
Sc9C Sc9C Sc2 65.7(4) 3_655 13
Pd2 Sc9C Sc2 135.5(4) . 5_554
Sc9C Sc9C Sc2 65.7(4) 3_655 5_554
Sc2 Sc9C Sc2 87.1(7) 13 5_554
Pd2 Sc9C Pd23 101.4(8) . .
Sc9C Sc9C Pd23 144.5(5) 3_655 .
Sc2 Sc9C Pd23 89.4(6) 13 .
Sc2 Sc9C Pd23 89.4(6) 5_554 .
Pd2 Sc9C Sc6 76.2(5) . 6_554
Sc9C Sc9C Sc6 96.6(4) 3_655 6_554
Sc2 Sc9C Sc6 147.3(9) 13 6_554
Sc2 Sc9C Sc6 60.25(13) 5_554 6_554
Pd23 Sc9C Sc6 91.6(4) . 6_554
Pd2 Sc9C Sc6 76.2(5) . 13
Sc9C Sc9C Sc6 96.6(4) 3_655 13
Sc2 Sc9C Sc6 60.25(13) 13 13
Sc2 Sc9C Sc6 147.3(9) 5_554 13
Pd23 Sc9C Sc6 91.6(4) . 13
Sc6 Sc9C Sc6 152.3(10) 6_554 13
Pd2 Sc9C Sc7 54.2(5) . 6_554
Sc9C Sc9C Sc7 67.8(4) 3_655 6_554
Sc2 Sc9C Sc7 129.5(7) 13 6_554
Sc2 Sc9C Sc7 91.1(4) 5_554 6_554
Pd23 Sc9C Sc7 141.1(6) . 6_554
Sc6 Sc9C Sc7 55.9(3) 6_554 6_554
Sc6 Sc9C Sc7 108.0(7) 13 6_554
Pd2 Sc9C Sc7 54.2(5) . 13
Sc9C Sc9C Sc7 67.8(4) 3_655 13
Sc2 Sc9C Sc7 91.1(4) 13 13
Sc2 Sc9C Sc7 129.5(7) 5_554 13
Pd23 Sc9C Sc7 141.1(6) . 13
Sc6 Sc9C Sc7 108.0(7) 6_554 13
Sc6 Sc9C Sc7 55.9(3) 13 13
Sc7 Sc9C Sc7 53.2(4) 6_554 13
Pd2 Sc9C Pd4 107.6(6) . 13
Sc9C Sc9C Pd4 117.5(4) 3_655 13
Sc2 Sc9C Pd4 51.9(3) 13 13
Sc2 Sc9C Pd4 110.8(8) 5_554 13
Pd23 Sc9C Pd4 46.5(3) . 13
Sc6 Sc9C Pd4 138.1(7) 6_554 13
Sc6 Sc9C Pd4 51.26(16) 13 13
Sc7 Sc9C Pd4 157.9(7) 6_554 13
Sc7 Sc9C Pd4 107.10(19) 13 13
Pd2 Sc9C Pd4 107.6(6) . 6_554
Sc9C Sc9C Pd4 117.5(4) 3_655 6_554
Sc2 Sc9C Pd4 110.8(8) 13 6_554
Sc2 Sc9C Pd4 51.9(3) 5_554 6_554
Pd23 Sc9C Pd4 46.5(3) . 6_554
Sc6 Sc9C Pd4 51.26(16) 6_554 6_554
Sc6 Sc9C Pd4 138.1(7) 13 6_554
Sc7 Sc9C Pd4 107.10(19) 6_554 6_554
Sc7 Sc9C Pd4 157.9(7) 13 6_554
Pd4 Sc9C Pd4 89.8(6) 13 6_554
Pd2 Sc9C Sc13 96.3(7) . .
Sc9C Sc9C Sc13 149.6(5) 3_655 .
Sc2 Sc9C Sc13 93.0(6) 13 .
Sc2 Sc9C Sc13 93.0(6) 5_554 .
Pd23 Sc9C Sc13 5.07(9) . .
Sc6 Sc9C Sc13 90.4(4) 6_554 .
Sc6 Sc9C Sc13 90.4(4) 13 .
Sc7 Sc9C Sc13 137.4(6) 6_554 .
Sc7 Sc9C Sc13 137.4(6) 13 .
Pd4 Sc9C Sc13 47.9(3) 13 .
Pd4 Sc9C Sc13 47.9(3) 6_554 .
Pd2 Sc10 Pd3 159.99(2) . .
Pd2 Sc10 Sc4 109.48(2) . .
Pd3 Sc10 Sc4 50.696(16) . .
Pd2 Sc10 Sc6 71.516(15) . 13
Pd3 Sc10 Sc6 121.48(2) . 13
Sc4 Sc10 Sc6 143.23(2) . 13
Pd2 Sc10 Sc1 50.088(16) . .
Pd3 Sc10 Sc1 110.00(2) . .
Sc4 Sc10 Sc1 59.40(2) . .
Sc6 Sc10 Sc1 110.91(2) 13 .
Pd2 Sc10 Sc12 144.43(2) . 13
Pd3 Sc10 Sc12 53.838(17) . 13
Sc4 Sc10 Sc12 99.83(2) . 13
Sc6 Sc10 Sc12 96.75(2) 13 13
Sc1 Sc10 Sc12 152.20(3) . 13
Pd2 Sc10 Sc11 56.189(14) . .
Pd3 Sc10 Sc11 114.61(2) . .
Sc4 Sc10 Sc11 89.28(2) . .
Sc6 Sc10 Sc11 59.955(16) 13 .
Sc1 Sc10 Sc11 58.295(16) . .
Sc12 Sc10 Sc11 145.90(3) 13 .
Pd2 Sc10 Sc10 56.860(11) . 10
Pd3 Sc10 Sc10 118.301(11) . 10
Sc4 Sc10 Sc10 88.548(16) . 10
Sc6 Sc10 Sc10 118.090(13) 13 10
Sc1 Sc10 Sc10 59.175(12) . 10
Sc12 Sc10 Sc10 105.644(18) 13 10
Sc11 Sc10 Sc10 107.389(13) . 10
Pd2 Sc10 Sc13 97.1(2) . .
Pd3 Sc10 Sc13 95.6(2) . .
Sc4 Sc10 Sc13 116.8(3) . .
Sc6 Sc10 Sc13 99.1(3) 13 .
Sc1 Sc10 Sc13 119.18(2) . .
Sc12 Sc10 Sc13 50.48(14) 13 .
Sc11 Sc10 Sc13 149.0(3) . .
Sc10 Sc10 Sc13 60.071(9) 10 .
Pd2 Sc10 Sc6 113.61(2) . .
Pd3 Sc10 Sc6 56.434(14) . .
Sc4 Sc10 Sc6 58.334(18) . .
Sc6 Sc10 Sc6 86.909(19) 13 .
Sc1 Sc10 Sc6 86.056(18) . .
Sc12 Sc10 Sc6 98.64(2) 13 .
Sc11 Sc10 Sc6 58.601(16) . .
Sc10 Sc10 Sc6 141.943(13) 10 .
Sc13 Sc10 Sc6 148.91(17) . .
Pd2 Sc10 Sc9B 50.8(4) . .
Pd3 Sc10 Sc9B 147.3(4) . .
Sc4 Sc10 Sc9B 148.5(3) . .
Sc6 Sc10 Sc9B 61.2(3) 13 .
Sc1 Sc10 Sc9B 96.9(3) . .
Sc12 Sc10 Sc9B 93.9(4) 13 .
Sc11 Sc10 Sc9B 95.1(4) . .
Sc10 Sc10 Sc9B 60.3(3) 10 .
Sc13 Sc10 Sc9B 53.9(5) . .
Sc6 Sc10 Sc9B 146.9(3) . .
Pd2 Sc10 Sc8 116.598(18) . .
Pd3 Sc10 Sc8 59.163(11) . .
Sc4 Sc10 Sc8 59.81(2) . .
Sc6 Sc10 Sc8 154.49(3) 13 .
Sc1 Sc10 Sc8 90.40(2) . .
Sc12 Sc10 Sc8 62.10(2) 13 .
Sc11 Sc10 Sc8 145.37(3) . .
Sc10 Sc10 Sc8 60.422(10) 10 .
Sc13 Sc10 Sc8 57.0(3) . .
Sc6 Sc10 Sc8 109.15(2) . .
Sc9B Sc10 Sc8 103.8(3) . .
Pd2 Sc11 Sc12 143.40(2) . .
Pd2 Sc11 Sc7 54.978(17) . 13
Sc12 Sc11 Sc7 90.38(2) . 13
Pd2 Sc11 Sc1 50.805(16) . .
Sc12 Sc11 Sc1 146.31(2) . .
Sc7 Sc11 Sc1 102.60(2) 13 .
Pd2 Sc11 Pd4 160.86(2) . .
Sc12 Sc11 Pd4 52.409(18) . .
Sc7 Sc11 Pd4 142.75(2) 13 .
Sc1 Sc11 Pd4 110.11(2) . .
Pd2 Sc11 Sc5 109.06(2) . .
Sc12 Sc11 Sc5 97.63(2) . .
Sc7 Sc11 Sc5 153.49(3) 13 .
Sc1 Sc11 Sc5 58.253(19) . .
Pd4 Sc11 Sc5 51.885(16) . .
Pd2 Sc11 Sc6 116.91(2) . .
Sc12 Sc11 Sc6 98.31(2) . .
Sc7 Sc11 Sc6 145.97(3) 13 .
Sc1 Sc11 Sc6 88.159(19) . .
Pd4 Sc11 Sc6 54.329(13) . .
Sc5 Sc11 Sc6 57.740(16) . .
Pd2 Sc11 Sc6 71.269(16) . 13
Sc12 Sc11 Sc6 102.48(2) . 13
Sc7 Sc11 Sc6 58.53(2) 13 13
Sc1 Sc11 Sc6 110.85(2) . 13
Pd4 Sc11 Sc6 121.49(2) . 13
Sc5 Sc11 Sc6 142.00(2) . 13
Sc6 Sc11 Sc6 87.445(19) . 13
Pd2 Sc11 Pd5 91.011(16) . .
Sc12 Sc11 Pd5 53.671(19) . .
Sc7 Sc11 Pd5 49.067(16) 13 .
Sc1 Sc11 Pd5 113.90(2) . .
Pd4 Sc11 Pd5 99.950(17) . .
Sc5 Sc11 Pd5 118.204(18) . .
Sc6 Sc11 Pd5 151.92(2) . .
Sc6 Sc11 Pd5 99.642(17) 13 .
Pd2 Sc11 Sc10 57.201(15) . .
Sc12 Sc11 Sc10 150.25(2) . .
Sc7 Sc11 Sc10 96.62(2) 13 .
Sc1 Sc11 Sc10 59.660(19) . .
Pd4 Sc11 Sc10 114.902(19) . .
Sc5 Sc11 Sc10 88.877(18) . .
Sc6 Sc11 Sc10 60.963(16) . .
Sc6 Sc11 Sc10 58.527(16) 13 .
Pd5 Sc11 Sc10 144.79(2) . .
Pd2 Sc11 Sc3 57.504(11) . .
Sc12 Sc11 Sc3 99.29(2) . .
Sc7 Sc11 Sc3 63.99(2) 13 .
Sc1 Sc11 Sc3 60.95(2) . .
Pd4 Sc11 Sc3 117.920(18) . .
Sc5 Sc11 Sc3 89.73(2) . .
Sc6 Sc11 Sc3 144.74(3) . .
Sc6 Sc11 Sc3 117.91(2) 13 .
Pd5 Sc11 Sc3 52.951(19) . .
Sc10 Sc11 Sc3 109.79(2) . .
Pd2 Sc11 Sc11 116.127(12) . 11
Sc12 Sc11 Sc11 57.871(13) . 11
Sc7 Sc11 Sc11 106.258(17) 13 11
Sc1 Sc11 Sc11 88.530(17) . 11
Pd4 Sc11 Sc11 58.513(10) . 11
Sc5 Sc11 Sc11 58.899(12) . 11
Sc6 Sc11 Sc11 106.203(14) . 11
Sc6 Sc11 Sc11 156.929(13) 13 11
Pd5 Sc11 Sc11 59.758(10) . 11
Sc10 Sc11 Sc11 144.438(13) . 11
Sc3 Sc11 Sc11 59.915(10) . 11
Pd4 Sc12 Sc13 63.6(3) . 13
Pd4 Sc12 Pd3 121.017(16) . 13
Sc13 Sc12 Pd3 113.94(13) 13 13
Pd4 Sc12 Pd3 121.017(16) . 14_545
Sc13 Sc12 Pd3 113.94(12) 13 14_545
Pd3 Sc12 Pd3 113.04(3) 13 14_545
Pd4 Sc12 Pd5 121.47(3) . .
Sc13 Sc12 Pd5 175.0(3) 13 .
Pd3 Sc12 Pd5 64.085(17) 13 .
Pd3 Sc12 Pd5 64.085(17) 14_545 .
Pd4 Sc12 Sc12 178.88(2) . 2_655
Sc13 Sc12 Sc12 115.3(3) 13 2_655
Pd3 Sc12 Sc12 59.246(15) 13 2_655
Pd3 Sc12 Sc12 59.246(15) 14_545 2_655
Pd5 Sc12 Sc12 59.647(17) . 2_655
Pd4 Sc12 Pd23 54.0(3) . 13
Sc13 Sc12 Pd23 9.56(7) 13 13
Pd3 Sc12 Pd23 117.53(9) 13 13
Pd3 Sc12 Pd23 117.53(9) 14_545 13
Pd5 Sc12 Pd23 175.5(3) . 13
Sc12 Sc12 Pd23 124.9(3) 2_655 13
Pd4 Sc12 Sc11 64.85(2) . .
Sc13 Sc12 Sc11 117.8(2) 13 .
Pd3 Sc12 Sc11 68.354(16) 13 .
Pd3 Sc12 Sc11 121.22(3) 14_545 .
Pd5 Sc12 Sc11 66.24(2) . .
Sc12 Sc12 Sc11 116.054(18) 2_655 .
Pd23 Sc12 Sc11 110.1(2) 13 .
Pd4 Sc12 Sc11 64.85(2) . 11
Sc13 Sc12 Sc11 117.8(2) 13 11
Pd3 Sc12 Sc11 121.22(3) 13 11
Pd3 Sc12 Sc11 68.353(16) 14_545 11
Pd5 Sc12 Sc11 66.24(2) . 11
Sc12 Sc12 Sc11 116.053(18) 2_655 11
Pd23 Sc12 Sc11 110.1(2) 13 11
Sc11 Sc12 Sc11 64.26(3) . 11
Pd4 Sc12 Sc10 67.640(17) . 7_545
Sc13 Sc12 Sc10 66.16(8) 13 7_545
Pd3 Sc12 Sc10 170.89(3) 13 7_545
Pd3 Sc12 Sc10 60.529(11) 14_545 7_545
Pd5 Sc12 Sc10 114.979(18) . 7_545
Sc12 Sc12 Sc10 112.039(17) 2_655 7_545
Pd23 Sc12 Sc10 64.17(5) 13 7_545
Sc11 Sc12 Sc10 120.14(3) . 7_545
Sc11 Sc12 Sc10 63.816(16) 11 7_545
Pd4 Sc12 Sc10 67.640(17) . 13
Sc13 Sc12 Sc10 66.16(8) 13 13
Pd3 Sc12 Sc10 60.529(11) 13 13
Pd3 Sc12 Sc10 170.89(3) 14_545 13
Pd5 Sc12 Sc10 114.979(18) . 13
Sc12 Sc12 Sc10 112.039(17) 2_655 13
Pd23 Sc12 Sc10 64.17(5) 13 13
Sc11 Sc12 Sc10 63.816(16) . 13
Sc11 Sc12 Sc10 120.14(3) 11 13
Sc10 Sc12 Sc10 124.96(3) 7_545 13
Pd4 Sc12 Sc8 114.66(3) . 13
Sc13 Sc12 Sc8 60.8(2) 13 13
Pd3 Sc12 Sc8 60.458(18) 13 13
Pd3 Sc12 Sc8 111.05(3) 14_545 13
Pd5 Sc12 Sc8 115.04(2) . 13
Sc12 Sc12 Sc8 64.419(15) 2_655 13
Pd23 Sc12 Sc8 68.7(2) 13 13
Sc11 Sc12 Sc8 117.14(2) . 13
Sc11 Sc12 Sc8 178.32(3) 11 13
Sc10 Sc12 Sc8 114.50(3) 7_545 13
Sc10 Sc12 Sc8 60.560(19) 13 13
Pd23 Sc13 Sc12 115.3(3) . 6_554
Pd23 Sc13 Sc12 115.3(3) . 13
Sc12 Sc13 Sc12 129.4(6) 6_554 13
Pd23 Sc13 Pd4 57.3(3) . 13
Sc12 Sc13 Pd4 172.6(6) 6_554 13
Sc12 Sc13 Pd4 58.06(4) 13 13
Pd23 Sc13 Pd4 57.3(3) . 6_554
Sc12 Sc13 Pd4 58.06(4) 6_554 6_554
Sc12 Sc13 Pd4 172.6(6) 13 6_554
Pd4 Sc13 Pd4 114.5(5) 13 6_554
Pd23 Sc13 Sc9B 30.6(6) . .
Sc12 Sc13 Sc9B 111.6(3) 6_554 .
Sc12 Sc13 Sc9B 111.6(3) 13 .
Pd4 Sc13 Sc9B 62.2(3) 13 .
Pd4 Sc13 Sc9B 62.2(3) 6_554 .
Pd23 Sc13 Sc9B 30.6(6) . 11_565
Sc12 Sc13 Sc9B 111.6(3) 6_554 11_565
Sc12 Sc13 Sc9B 111.6(3) 13 11_565
Pd4 Sc13 Sc9B 62.2(3) 13 11_565
Pd4 Sc13 Sc9B 62.2(3) 6_554 11_565
Sc9B Sc13 Sc9B 61.1(11) . 11_565
Pd23 Sc13 Sc8 146.89(16) . .
Sc12 Sc13 Sc8 69.0(3) 6_554 .
Sc12 Sc13 Sc8 69.0(3) 13 .
Pd4 Sc13 Sc8 116.94(16) 13 .
Pd4 Sc13 Sc8 116.94(16) 6_554 .
Sc9B Sc13 Sc8 116.3(5) . .
Sc9B Sc13 Sc8 177.4(6) 11_565 .
Pd23 Sc13 Sc8 146.89(16) . 9_565
Sc12 Sc13 Sc8 69.0(3) 6_554 9_565
Sc12 Sc13 Sc8 69.0(3) 13 9_565
Pd4 Sc13 Sc8 116.94(16) 13 9_565
Pd4 Sc13 Sc8 116.94(16) 6_554 9_565
Sc9B Sc13 Sc8 177.4(6) . 9_565
Sc9B Sc13 Sc8 116.3(5) 11_565 9_565
Sc8 Sc13 Sc8 66.2(3) . 9_565
Pd23 Sc13 Sc10 89.7(3) . .
Sc12 Sc13 Sc10 117.0(2) 6_554 .
Sc12 Sc13 Sc10 63.36(6) 13 .
Pd4 Sc13 Sc10 64.98(9) 13 .
Pd4 Sc13 Sc10 114.6(2) 6_554 .
Sc9B Sc13 Sc10 63.5(5) . .
Sc9B Sc13 Sc10 115.8(6) 11_565 .
Sc8 Sc13 Sc10 62.07(14) . .
Sc8 Sc13 Sc10 118.6(4) 9_565 .
Pd23 Sc13 Sc10 89.7(3) . 11_565
Sc12 Sc13 Sc10 117.0(2) 6_554 11_565
Sc12 Sc13 Sc10 63.36(6) 13 11_565
Pd4 Sc13 Sc10 64.98(9) 13 11_565
Pd4 Sc13 Sc10 114.6(2) 6_554 11_565
Sc9B Sc13 Sc10 115.8(6) . 11_565
Sc9B Sc13 Sc10 63.5(5) 11_565 11_565
Sc8 Sc13 Sc10 118.6(4) . 11_565
Sc8 Sc13 Sc10 62.07(14) 9_565 11_565
Sc10 Sc13 Sc10 120.14(2) . 11_565
Pd23 Sc13 Sc10 89.7(3) . 10
Sc12 Sc13 Sc10 63.36(6) 6_554 10
Sc12 Sc13 Sc10 117.0(2) 13 10
Pd4 Sc13 Sc10 114.6(2) 13 10
Pd4 Sc13 Sc10 64.98(9) 6_554 10
Sc9B Sc13 Sc10 63.5(5) . 10
Sc9B Sc13 Sc10 115.8(6) 11_565 10
Sc8 Sc13 Sc10 62.07(14) . 10
Sc8 Sc13 Sc10 118.6(4) 9_565 10
Sc10 Sc13 Sc10 59.860(19) . 10
Sc10 Sc13 Sc10 179.3(6) 11_565 10
Sc13 Pd23 Sc9B 143.0(7) . .
Sc13 Pd23 Sc9B 143.0(7) . 11_565
Sc9B Pd23 Sc9B 74.1(14) . 11_565
Sc13 Pd23 Pd4 112.5(3) . 13
Sc9B Pd23 Pd4 72.2(3) . 13
Sc9B Pd23 Pd4 72.2(3) 11_565 13
Sc13 Pd23 Pd4 112.5(3) . 6_554
Sc9B Pd23 Pd4 72.2(3) . 6_554
Sc9B Pd23 Pd4 72.2(3) 11_565 6_554
Pd4 Pd23 Pd4 135.0(7) 13 6_554
Sc13 Pd23 Sc9A 143.2(3) . .
Pd4 Pd23 Sc9A 72.2(3) 13 .
Pd4 Pd23 Sc9A 72.2(3) 6_554 .
Sc13 Pd23 Sc9A 143.2(3) . 11_565
Pd4 Pd23 Sc9A 72.2(3) 13 11_565
Pd4 Pd23 Sc9A 72.2(3) 6_554 11_565
Sc9A Pd23 Sc9A 73.6(7) . 11_565
Sc13 Pd23 Sc12 55.1(3) . 6_554
Sc9B Pd23 Sc12 117.2(3) . 6_554
Sc9B Pd23 Sc12 117.2(3) 11_565 6_554
Pd4 Pd23 Sc12 167.6(6) 13 6_554
Pd4 Pd23 Sc12 57.37(8) 6_554 6_554
Sc9A Pd23 Sc12 117.25(15) . 6_554
Sc9A Pd23 Sc12 117.25(15) 11_565 6_554
Sc13 Pd23 Sc12 55.1(3) . 13
Sc9B Pd23 Sc12 117.2(3) . 13
Sc9B Pd23 Sc12 117.2(3) 11_565 13
Pd4 Pd23 Sc12 57.37(8) 13 13
Pd4 Pd23 Sc12 167.6(6) 6_554 13
Sc9A Pd23 Sc12 117.25(15) . 13
Sc9A Pd23 Sc12 117.25(15) 11_565 13
Sc12 Pd23 Sc12 110.3(5) 6_554 13
Sc13 Pd23 Sc9C 144.5(5) . 11_565
Pd4 Pd23 Sc9C 71.8(3) 13 11_565
Pd4 Pd23 Sc9C 71.8(3) 6_554 11_565
Sc12 Pd23 Sc9C 117.7(2) 6_554 11_565
Sc12 Pd23 Sc9C 117.7(2) 13 11_565
Sc13 Pd23 Sc9C 144.5(5) . .
Pd4 Pd23 Sc9C 71.8(3) 13 .
Pd4 Pd23 Sc9C 71.8(3) 6_554 .
Sc12 Pd23 Sc9C 117.7(2) 6_554 .
Sc12 Pd23 Sc9C 117.7(2) 13 .
Sc9C Pd23 Sc9C 71.0(11) 11_565 .
Sc13 Pd23 Sc10 80.6(3) . .
Sc9B Pd23 Sc10 67.3(6) . .
Sc9B Pd23 Sc10 130.2(6) 11_565 .
Pd4 Pd23 Sc10 66.879(19) 13 .
Pd4 Pd23 Sc10 121.13(11) 6_554 .
Sc9A Pd23 Sc10 67.5(3) . .
Sc9A Pd23 Sc10 130.0(5) 11_565 .
Sc12 Pd23 Sc10 108.1(3) 6_554 .
Sc12 Pd23 Sc10 60.21(12) 13 .
Sc9C Pd23 Sc10 129.0(6) 11_565 .
Sc9C Pd23 Sc10 68.6(5) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Pd1 Sc5 2.9415(7) 9
Pd1 Sc5 2.9415(7) 10
Pd1 Sc5 2.9415(7) 2
Pd1 Sc5 2.9415(7) .
Pd1 Sc1 2.9929(8) 9
Pd1 Sc1 2.9929(8) 3
Pd1 Sc1 2.9929(8) 11
Pd1 Sc1 2.9929(8) .
Pd1 Sc4 3.0445(8) .
Pd1 Sc4 3.0446(8) 9
Pd1 Sc4 3.0446(8) 10
Pd1 Sc4 3.0446(8) 2
Pd2 Sc9C 2.57(3) .
Pd2 Sc9A 2.594(15) .
Pd2 Sc1 2.6399(8) .
Pd2 Sc9B 2.73(3) .
Pd2 Sc7 2.8353(5) 13
Pd2 Sc7 2.8353(5) 6_554
Pd2 Sc11 2.9753(6) 10
Pd2 Sc11 2.9753(6) .
Pd2 Sc10 3.0100(6) 10
Pd2 Sc10 3.0100(6) .
Pd2 Sc3 3.0317(4) .
Pd3 Sc4 2.6792(8) .
Pd3 Sc7 2.7592(8) .
Pd3 Sc12 2.8563(6) 13
Pd3 Sc12 2.8563(5) 14_455
Pd3 Sc6 3.0247(6) 12
Pd3 Sc6 3.0247(6) .
Pd3 Pd5 3.0491(4) 13
Pd3 Sc10 3.0801(6) .
Pd3 Sc10 3.0801(6) 12
Pd3 Sc8 3.1738(4) .
Pd3 Sc11 3.3581(6) 13
Pd3 Sc11 3.3581(6) 8_455
Pd4 Pd23 2.663(6) 13
Pd4 Sc12 2.7720(9) .
Pd4 Sc5 2.7862(8) .
Pd4 Sc6 2.9186(6) 11
Pd4 Sc6 2.9186(6) .
Pd4 Sc2 2.9190(4) .
Pd4 Sc13 2.925(9) 13
Pd4 Sc9B 3.064(14) 13
Pd4 Sc9B 3.064(14) 7_545
Pd4 Sc11 3.1666(6) .
Pd4 Sc11 3.1667(6) 11
Pd4 Sc9A 3.281(13) 13
Pd5 Sc7 2.6770(8) 14_545
Pd5 Sc7 2.6769(8) 13
Pd5 Sc12 2.8905(10) 2_655
Pd5 Sc12 2.8905(10) .
Pd5 Sc3 2.9350(7) .
Pd5 Sc3 2.9350(7) 9_655
Pd5 Pd3 3.0491(4) 13
Pd5 Pd3 3.0491(4) 14_545
Pd5 Sc11 3.2838(5) .
Pd5 Sc11 3.2839(5) 12_655
Pd5 Sc11 3.2839(5) 11
Pd5 Sc11 3.2839(5) 2_655
Sc1 Sc5 3.0995(8) 10
Sc1 Sc5 3.0995(8) .
Sc1 Sc1 3.1455(15) 11
Sc1 Sc4 3.1642(8) .
Sc1 Sc4 3.1642(8) 10
Sc1 Sc11 3.1655(7) 10
Sc1 Sc11 3.1656(7) .
Sc1 Sc10 3.2112(9) 10
Sc1 Sc10 3.2113(9) .
Sc1 Sc3 3.2810(12) .
Sc2 Pd4 2.9191(4) 2
Sc2 Sc9C 3.14(2) 13
Sc2 Sc9C 3.14(2) 15_455
Sc2 Sc9C 3.14(2) 7_545
Sc2 Sc9C 3.14(2) 5_445
Sc2 Sc5 3.1610(11) .
Sc2 Sc5 3.1610(11) 2
Sc2 Sc9A 3.204(10) 13
Sc2 Sc9A 3.204(10) 15_455
Sc2 Sc9A 3.204(10) 5_445
Sc2 Sc9A 3.204(10) 7_545
Sc3 Pd5 2.9350(7) 9_655
Sc3 Pd2 3.0317(4) 11
Sc3 Sc1 3.2810(12) 11
Sc3 Sc11 3.2995(6) 4
Sc3 Sc11 3.2995(6) 10
Sc3 Sc11 3.2995(6) 11
Sc3 Sc11 3.2995(6) .
Sc3 Sc3 3.421(2) 9_655
Sc3 Sc7 3.4231(9) 13
Sc4 Sc4 3.1301(14) 10
Sc4 Sc6 3.1593(8) 12
Sc4 Sc6 3.1594(8) .
Sc4 Sc1 3.1642(8) 3
Sc4 Sc10 3.1749(7) .
Sc4 Sc10 3.1749(7) 12
Sc4 Sc5 3.1841(8) 2
Sc4 Sc5 3.1841(8) .
Sc4 Sc8 3.2478(12) .
Sc5 Sc1 3.0995(8) 11
Sc5 Sc6 3.1032(7) 11
Sc5 Sc6 3.1033(7) .
Sc5 Sc5 3.1430(15) 2
Sc5 Sc4 3.1841(8) 2
Sc5 Sc11 3.2020(8) .
Sc5 Sc11 3.2020(8) 11
Sc6 Sc7 3.1266(9) .
Sc6 Sc10 3.1890(7) 13
Sc6 Sc11 3.2252(7) .
Sc6 Sc11 3.2367(8) 13
Sc6 Sc9C 3.241(7) 13
Sc6 Sc9A 3.252(4) 13
Sc6 Sc10 3.3036(7) .
Sc7 Pd5 2.6769(8) 13
Sc7 Pd2 2.8352(5) 13
Sc7 Pd2 2.8352(5) 15_455
Sc7 Sc7 3.0669(15) 10_556
Sc7 Sc6 3.1266(9) 12
Sc7 Sc11 3.1572(6) 8_455
Sc7 Sc11 3.1572(6) 13
Sc7 Sc9C 3.42(3) 15_455
Sc7 Sc9C 3.42(2) 13
Sc7 Sc3 3.4230(9) 13
Sc8 Sc13 3.164(14) 9_565
Sc8 Sc13 3.164(14) .
Sc8 Pd3 3.1739(4) 10
Sc8 Sc4 3.2478(12) 10
Sc8 Sc10 3.3335(7) .
Sc8 Sc10 3.3336(7) 3
Sc8 Sc10 3.3336(7) 12
Sc8 Sc10 3.3336(7) 10
Sc8 Sc12 3.3828(9) 13
Sc8 Sc12 3.3828(9) 14_455
Sc9A Pd23 2.90(2) .
Sc9A Sc9A 3.20(4) 3_655
Sc9A Sc2 3.204(10) 13
Sc9A Sc2 3.204(10) 5_554
Sc9A Sc6 3.252(4) 6_554
Sc9A Sc6 3.252(4) 13
Sc9A Pd4 3.281(13) 13
Sc9A Pd4 3.281(13) 6_554
Sc9A Sc13 3.37(2) .
Sc9A Sc9A 3.47(3) 11_565
Sc9A Sc10 3.489(14) 10
Sc9B Pd23 2.53(3) .
Sc9B Sc13 3.00(3) .
Sc9B Sc9B 3.05(5) 11_565
Sc9B Pd4 3.064(14) 13
Sc9B Pd4 3.064(14) 6_554
Sc9B Sc2 3.26(2) 13
Sc9B Sc2 3.26(2) 5_554
Sc9B Sc6 3.319(8) 6_554
Sc9B Sc6 3.319(8) 13
Sc9B Sc10 3.33(3) 10
Sc9B Sc10 3.33(3) .
Sc9C Sc9C 2.59(5) 3_655
Sc9C Sc2 3.14(2) 13
Sc9C Sc2 3.14(2) 5_554
Sc9C Pd23 3.23(3) .
Sc9C Sc6 3.241(7) 6_554
Sc9C Sc6 3.241(7) 13
Sc9C Sc7 3.42(2) 6_554
Sc9C Sc7 3.42(2) 13
Sc9C Pd4 3.487(19) 13
Sc9C Pd4 3.487(19) 6_554
Sc9C Sc13 3.70(3) .
Sc10 Sc6 3.1891(7) 13
Sc10 Sc12 3.2227(7) 13
Sc10 Sc11 3.2867(8) .
Sc10 Sc10 3.2910(11) 10
Sc10 Sc13 3.2980(6) .
Sc11 Sc12 3.1098(9) .
Sc11 Sc7 3.1572(6) 13
Sc11 Sc6 3.2368(8) 13
Sc11 Sc11 3.3079(11) 11
Sc12 Sc13 2.782(7) 13
Sc12 Pd3 2.8563(6) 13
Sc12 Pd3 2.8563(6) 14_545
Sc12 Sc12 2.9212(17) 2_655
Sc12 Pd23 3.065(9) 13
Sc12 Sc11 3.1099(9) 11
Sc12 Sc10 3.2228(7) 7_545
Sc12 Sc10 3.2228(7) 13
Sc12 Sc8 3.3828(9) 13
Sc13 Pd23 0.563(3) .
Sc13 Sc12 2.782(7) 6_554
Sc13 Sc12 2.782(7) 13
Sc13 Pd4 2.925(9) 13
Sc13 Pd4 2.925(9) 6_554
Sc13 Sc9B 3.00(3) 11_565
Sc13 Sc8 3.164(14) 9_565
Sc13 Sc10 3.2980(6) 11_565
Sc13 Sc10 3.2980(6) 10
Pd23 Sc9B 2.53(3) 11_565
Pd23 Pd4 2.663(6) 13
Pd23 Pd4 2.663(6) 6_554
Pd23 Sc9A 2.90(2) 11_565
Pd23 Sc12 3.065(9) 6_554
Pd23 Sc12 3.065(9) 13
Pd23 Sc9C 3.23(3) 11_565
